Effects of the synthetic method on the particle
size and purity of magnetite
Efecto del método de síntesis en el tamaño de
partícula y pureza de la magnetita
Beatriz Jaramillo Tabares, Alejandro Alberto Zuleta Gil, Franklin Jaramillo Isaza*
Grupo de Corrosión y Protección (GCP), Universidad de Antioquia, calle 62 N.º 52-59, SIU, Torre 2, Laboratorio 330,Medellín, Colombia.
(Recibido el 10 de febrero de 2009. Aceptado el 24 de agosto de 2009)
The characterization of magnetites synthesized by methods reported with
some modiications is presented. The inluence on purity and particle size
of the obtained oxides is discussed. The samples were characterized by Mössbauer Spectroscopy at room temperature, particle size analysis by light scattering and by transmission electron microscopy of naked particles. The results showed that depending on the method of synthesis there are variations on stoichiometry and composition of magnetites, being this difference more important when the rate of addition of the alkaline solution to the combined ferrous and dispersant solution is changed. Moreover, it has been found strong agglomeration evidenced by TEM, however the sizes of the individual crystallites are in the nanometer scale.
--- Keywords: Magnetite synthesis, nanometric magnetite, magnetite characterization
Se presenta la evaluación de magnetitas sintetizadas bajo diferentes condiciones
reportadas en la literatura y con algunas modiicaciones, su inluencia en la
pureza y en el tamaño de partícula de los óxidos obtenidos. Las muestras se caracterizaron mediante espectroscopía Mössbauer a temperatura ambiente, análisis por dispersión de luz y microscopía electrónica de transmisión. Los resultados Mössbauer mostraron variaciones estequiométricas y de composición, que fueron más notables cuando una combinación de solución ferrosa y dispersante se agregó rápidamente a una solución alcalina. Además,
se encontró que el tamaño de partícula también cambia dependiendo del método de síntesis.
--- Palabras clave: Síntesis de magnetita, espectroscopía Mössbauer, tamaño de partícula, magnetita nanoparticulada
Magnetite (Fe3O4) is a ferromagentic oxide widely studied due to its broad range of applications
such as ferroluid, pigment, storage information
material, biomedical applications, catalyst, among others [1-5]. It has been found that magnetite nanoparticles show superparamagnetic behavior and their properties are strongly
inluenced by the method of synthesis. The main
reported methods are sonochemical , chemical co-precipitation [7-9]forced hydrolysis reaction , micro-emulsion , hydrothermal [12-14], pyrolysis  and electrochemical synthesis . Moreover there are some studies [17,18] related to the effect of pH, temperature and stirring conditions in purity, stoichiometry and particle size variations of synthetic magnetites.
Magnetite has an inverse spinel structure, with a face-centred cubic unit cell based on 32 O2- that contain 8 Fe3+ ions on the tetrahedral sites (A sites) and 16 Fe ions on the octahedral sites (B sites); 8 of which are Fe2+ end the other 8 are Fe3+. Its formula is written as Y[XY]O4 where X=Fe2+, Y=Fe3+ and the brackets denote octahedral sites . At room temperature the Mössbauer spectrum of magnetite shows two magnetic components. A sextet corresponding to Fe3+ on
the tetrahedral sites (A), with higher hyperine ield and a sextet with lower hyperine ield due
to Fe2,5+ on the octahedral sites (B).
The lines corresponding to B-sites are broader and larger than A-sites because of hopping of electrons between Fe2+ and Fe3+ ions occurs only on the B-sites, leading to the well known “Fe2,5+”
ionic state . A simpliied formula of magnetite
can be written as Fe3-xO4, where the oxidation parameter xcan vary continuously from zero, for a stoichiometric magnetite, to 1/
3 for maghemite
(γ-Fe2O3). This parameter can be calculated from
the Mössbauer spectra using the expression
x=(2R-1.06)/(5.3+6R), where R represents the ratio of the subspectral area of the A sites to the subspectral area of B sites.
The properties of magnetite are strongly inluenced
by particle size, purity and stoichiometry. Most of the recent applications reported in the literature have taken advantage of the nanometric size. However, many of those papers focus mainly on the size rather than stoichiometry or purity of the oxides, and problems like the formation of other phases as maghemite and goethite in the synthesis of magnetite are poorly discussed. In
the present work the inluence of modiications
on the purity and stoichiometry of the oxides in the conventional synthetic hydrothermal method
is studied. Such modiications include addition
rate and order of the precursors, and usage of dispersant. An improvement on the hydrothermal method is presented in order to obtain a balance between size and purity.
FeCl2.4H2O and FeCl3.6H2O (Merck), NaOH (Carlo Erba) and NaNO3 (Merck), polyethylene-glycol 4000 (Merck) were used without any further
puriication. The water used in all experiments was
de-ionized with conductivity 0.054 mScm−1.
Synthesis and characterization
Three different methods of synthesis were evaluated, with some variations in each of them
to inally obtain eight different magnetites. For a
the other way around. In some cases polyethylene-glycol (PEG) was used as a dispersant to increase the viscosity of the system and evaluate its
effect on the inal particle size of the oxides.
Stoichiometric quantities of the precursors were used and taken from the literature [7, 17]. Thus the precipitate obtained was decanted in a dialysis tubing cellulose membrane, and placed in a bath of distilled water. The anions of the suspension were removed by osmosis through the membrane. The water of the bath was replaced many times until the conductivity of the bath was
constant and similar to the deionised water (0.054 µS Scm−1). The resulting was iltered and dried at 40 ºC for 48 hours. The prepared samples were stored in a desiccator under nitrogen atmosphere. All the used methods are described on Table 1.
These are classiied on three groups, group 1
(M1) corresponding to chemical co-precipitation from Fe2+ and Fe3+, group 2 (M2, M2a y M2b), in which the oxidizing solution was added to the ferrous solution, and group 3 (M3, M3a, M3b, M3c) in which the ferrous solution was added to the oxidizing solution.
Table 1 Variables considered in simple preparation of the magnetites
Sample Variables considered
M1 Chemical co-precipitation from Fe
+2 and Fe+3 aqueous salt solutions, molar ratio of Fe+3:Fe+2 = 2:1, by
addition of NH4OH to control pH .
M2 Hydrothermal. The alkaline solution, NaNO3 and NaOH, is added dropwise and slowly to the ferrous
chloride solution .
M2a Hydrothermal. The alkaline solution, NaNO3 and NaOH, with PEG as a dispersant is added dropwise and
slowly to the ferrous chloride solution [11, 19].
M2b Hydrothermal. Adding dropwise and slowly the alkaline solution, NaNO3 and NaOH, with PEG to the
ferrous chloride solution also containing PEG.
M3 Hydrothermal. Adding the ferrous chloride solution dropwise and slowly to the alkaline solution, NaNO3
and NaOH 
M3a Hidrothermal. Adding the ferrous chloride solution dropwise and slowly to the alkaline solution, NaNO3
and NaOH, with PEG.
M3b Hydrothermal. Adding dropwise and slowly (0,8 mL/s) the ferrous chloride solution to the alkaline solution, NaNO3 and NaOH, with PEG[10, 11, 18]
M3c Hydrothermal. Adding dropwise but more quickly (1,6 mL/s) the ferrous chloride solution with to the alkaline solution, NaNO3 and NaOH, with PEG.
* When PEG is used, the ratio is 6 g PEG:1 g Fe total.
The samples of synthesized magnetites were characterized by Mössbauer spectroscopy at room temperature. Mössbauer spectra were obtained in the transmission mode using a constant acceleration with a Co/Rh source and a triangulate signal to control source velocity with constant
acceleration. The spectra were itted using
MOSF program which is based on a nonlinear least-square method assuming Lorentzian line
shapes. A three or four sextets model has been
used. The two irst attributed to magnetite,
with 1% of PEG. TEM images were obtained in a Tecnai 20 TW, D345, FP 5020 / 10 Phillips microscope at 200 kV and 25-30 mA.
Results and discussionResults showed different features on the inal
product comparing the synthesis obtained by hydrothermal and co-precipitation route. These variations are mainly attributable to solution mixing order.
The co-precipitation method (M1) normally gives a brownish solution when the reagents are mixed. As caution, the water used in solutions was degassed over 30 min. This color can remain
during all the reaction and inally give a
brown-like oxide. In contrast, the hydrothermal method with dropwise addition of alkaline/oxidizing solution to the ferrous solution (M2, M2a y M2b), with or without PEG presented the formation of a black suspension localized at the contact of the drop with the solution and homogenized
throughout out the lask while the reaction took
place. Finally, When the ferrous solution was added to the alkaline/oxidizing solution (M3, M3a, M3b y M3c), a suspended solid was also formed from the localized oxidation of Fe2+ to Fe3+, the suspension looked like green rusts that quickly change to black magnetite in the alkaline medium, this is in agreement with the results previously reported for this synthetic strategy .
According to the Mössbauer Spectra (Figure 1), all samples presented magnetite as the main component (see Table 2 for sextets 1 and
2). In all the ittings the hyperine parameters
corresponded to magnetite (Bhf1:49T, Bhf2:46
T, δ1:0.15mm/s, δ2:0.56mm/s) and goethite (Bhf1:38.2 T, δ1:0.25mm/s) . Sample M1 presented around 30% of a second phase (sextet 3) assigned to goethite according to the
characteristic hyperine parameters . Sample M2 was itting using a model with four sextets,
S1 and S2 corresponding to magnetite and sextets third and fourth corresponding to goethites of different particle size (see Figure 3b). Samples
M2a, M3a, M3b, M2b, M3c were itted using
a three sextets model. S1 and S2 correspond to magnetite and S3 corresponding to goethite.
Sample M3 was itted using two sextets (S1 and
S2) which correspond to a highly pure magnetite.
100.0 99.5 99.0 98.5 100.0 90.0 80.0 70.0 60.0 100.0 99.5 99.0 98.5 98.0 100.0 99.8 99.6 99.4 99.2 99.0 98.8 100.0 99.5 99.0 98.5 98.0 97.5 100.0 99.5 99.0 98.5 98.0 97.5 100.0 99.5 99.0 98.5 98.0 97.5 97.0 96.5 100.0 99.5 99.0 98.5 98.0 97.5
-10 -5 0 5 10 -10 -5 0 5 10
-10 -5 0 5 10 -10 -5 0 5 10
-10 -5 0 5 10 -10 -5 0 5 10
-10 -5 0 5 10 -10 -5 0 5 10
Velocity (mm/s )-1
Figure 1 Room temperature Mössbauer spectra of
synthetized magnetites. (a) M1, (b) M2, (c) M2a, (d) M2b, (e) M3, (f) M3a, (g) M3b, (h) M3c
Table 2 shows the calculated oxidation parameter
Table 2 Hyperine Parameters of synthetized magnetites
Sample Component Bhf (T) δ (mm/s) ΔEQ (mm/s) Area (%) x*
M1 Sextet 1 48.9 0.15 0.0 16.9 ±0.06
Sextet 2 45.9 0.54 0.0 53.2
Sextet 3 38.0 0.26 -0.27 29.9
M2 Sextet 1 48.7 0.26 0.0 47.0 0.073
Sextet 2 45.7 0.66 0.0 50.6
Sextet 3 38.6 0.26 -0.27 1.0
Sextet 4 28.1 0.27 -0.26 1.4
M2a Sextet 1 48.6 0.16 0.0 31.8 0.029
Sextet 2 45.8 0.56 0.0 47.8
Sextet 3 37.9 0.25 -0.21 20.3
M2b Sextet 1 48.5 0.28 0.0 41.4 0.050
Sextet 2 45.7 0.64 0.0 53.1
Sextet 3 37.4 0.25 -0.18 5.4
M3 Sextet 1 48.9 0.28 0.0 38.3 0.020
Sextet 2 45.7 0.67 0.0 61.7
M3a Sextet 1 49.0 0.16 0.0 39.8 0.103
Sextet 2 45.9 0.56 0.0 34.1
Sextet 3 38.5 0.25 0.0 29.1
M3b Sextet 1 49.0 0.16 0.0 35.7 0.012
Sextet 2 45.9 0.55 0.0 61.4
Sextet 3 37.7 0.26 -0.29 2.8
M3c Sextet 1 48.9 0.15 0.0 43.8 0.087
Sextet 2 46.0 0.55 0.0 42.4
Sextet 3 39.6 0.30 -0.18 13.8
*x: oxidation parameter. x = (2R-1.06)/(5.3+6R)
For clarity, igure 2 shows the amount of goethite
found in all the obtained samples calculated from the Mössbauer spectra (Figure 1 and Table 2). Remarkable differences in the amount of goethite were observed depending on the method of synthesis and the rate of addition of the reactive solutions. Method M1 gives the highest amount of goethite (~30%), probably due
to differences on co-precipitation kinetics of Fe2+ and Fe3+ ions, giving as result a stoichiometric changes in balance, which are favorable for
the oxi-hydroxide α-FeOOH formation. When
the ferrous solution (M2). Moreover, when a solution of PEG and oxidizing/alkaline (M2a and M3a) was used at 0.2 mL/s, independently of the order of addition, an increase on the amount of goethite was observed.
M1 M2 M2a M2b M3 M3a M3b M3c
Sample 30 25 20 15 10 5 0 Goethite amount (%)
Figure 2 Amount of goethite in samples
An increase of the viscosity seems to promote the oxidation process of Fe2+ to Fe3+ favoring the formation of additional phases like goethite. Further decrease in the amount of goethite (3%) was observed for an addition rate of 0.8 mL/s (M3b) and an increase up to about 14% was observed for M3c (1.6 mL/s).
It is worth noting that the methods M2 and M3, despite being very similar in terms of procedure, it appears that just changing the order in the addition of the solutions resulted in substantial changes in the stoichiometry and purity of the obtained magnetites. This may be due to the fact that on method M3 each drop of Fe2+ solution is oxidized immediately in the right ratio 1:2 upon making contact with the solution of NaOH and NaNO3. In method M2, by adding the oxidizing/ alkaline solution to the Fe2+, the transformation process is much localized at the top of the solution and the concentration of Fe2+ decreases in the surroundings of the drop. In this case more Fe2+ needs to contact the oxidizing agent in order to the reaction to take place gradually.
Figure 3 shows the particle size distribution obtained by light scattering from the dispersions. As the particles in ethanol/PEG were not completely
stable, this technique gave information mainly about aggregation and sizes of the bulky particles (see TEM below). Excepting samples M2a and M3a (alkaline/oxidative solution containing PEG and addition rate at 0.2 mL/s) the size distribution of the magnetites was bi- and tri-modal. In general, it was found particle sizes between 1 and 10 mm, being 1 mm the most common size. Samples M3b and M2b (Figure 3d and Figure 3g) showed particle size distributions between 0,1 and 1 mm, with greater percentage at 0,1 mm for the oxide obtained using method M3b. It may be noted that the way and rate of addition of solutions, as well as its composition
(with or without PEG), had inluence both in purity
of magnetite and in the size and aggregation of the particles. Samples without PEG (M1, M2, M3) showed particle size between 1 and 10 mm; however samples with PEG in the oxidizing/alkaline solution (M2a, M3a) exhibited particle sizes closer to 1 mm. On the other hand, samples with PEG in the ferrous solution gave particles sizes of 0,1 and 10 mm, being the smallest for those in which the solution was added slowly (M3b).
12 10 8 6 4 2 0
0.01 0.1 1 10 100 1000 10000
(a) 12 10 8 6 4 2 0
0.01 0.1 1 10 100 1000 1000
(b) 12 10 8 6 4 2 0
0.01 0.1 1 10 100 1000 10000
(c) 12 10 8 6 4 2 0
0.01 0.1 1 10 100 1000 10000
(e) 12 10 8 6 4 2 0
0.01 0.1 1 10 100 1000 10000
(g) 12 10 8 6 4 2 0
0.01 0.1 1 10 100 1000 10000
0.01 0.1 1 10 100 1000 10000 12 10 8 6 4 2 0 12 10 8 6 4 2 0
0.01 0.1 1 10 100 1000 10000
Particle size ( m)µ
Figure 3 Particle size distribution. (a) M1, (b) M2, (c)
Although the observed particle distribution by light scattering was found to be in the micrometer size due to aggregates, TEM images contribute to validate the individual size of the particles. Figure 4 shows the transmission electron micrographs of samples M1, M2a y M3b.
TEM images showed particle sizes much less than 100 nm for sample M1 (about 10 nm). This is in agreement with the literature for magnetites obtained from Fe2+ and Fe3+[17,24]. Particles at around 100 nm were obtained for sample M3b, similar to the result obtained by particle size distribution for the same sample. On light scattering analysis, the second peak is, in general, associated
to aggregation, as was also conirmed by TEM.
The individual particles of nano-magnetites tend to aggregate by formation of strong magnetic dipole-dipole interactions in order to reduce the surface energy of its high surface area/volume ratio . It has been suggested in the literature that the presence of PEG prevents the aggregation of nanoparticles into larger particles and could kinetically control the growth rates of various crystalline faces affecting the diffusion rate of Fe+3 on the surfaces of Fe
3O4 nanocrystallites and their epitaxial growth . As showed in Figure 4, for M2a and M3b, PEG helped to dispersed the magnetite particles in both cases, however in terms of particle size and distribution the order of addition of the reagents had a more important effect for each sample, as observed by TEM and light scattering.
150 nm 150 nm 150 nm
Figure 4 TEM images. (a) M1, (b) M2a, (c) M3b
It was veriied, that the order and rate of addition
of the reactive solutions and the presence of PEG as dispersant has a major effect on the purity, stoichiometry and particle size of the obtained oxides. In general, as expected, the size of the particles decreased when used PEG as dispersant; however its presence affected the purity of the oxides and favored the formation of goethite. Highly pure magnetite was obtained by adding the iron solution on the alkaline/oxidizing (M3), however for this sample the average particle size is expected to be higher than 200nm according to the
light scattering measurements. On the other hand the magnetite M3b obtained by adding the ferrous solution to the alkaline/oxidizing solution with PEG presented both interesting particle size (higher than 40 nm) and relative good purity (about 2.8% of goethite). Even though co-precipitation method (M1, Fe2+/Fe3+), exhibited smallest particle size (~ 10 nm), from Mössbauer analysis can be deduced that is not a highly pure magnetite.
AcknowledgementsThe authors wish to acknowledge inancial
1. R. Y. Hong, T. T. Pan, Y. P. Han, H. Z. Li, J. Ding, S.
Hand. “Magnetic ield synthesis of Fe3O4 nanoparticles
used as a precursor of ferroluids”. J. Magn. Mater. Vol. 310. 2007. pp. 37-47.
2. M. A. Legodi, D. de Waal. “The preparation of
magnetite, goethite, hematite and maghemite of
pigment quality from mill scale iron waste”. Dyes and
Pigments. Vol. 74. 2007. pp. 161-168.
3. S. Sun, C. B. Murray, D. Weller, L. Folks, A. Moser.
“Monodisperse FePt Nanoparticles and Ferromagnetic
FePt Nanocrystal Superlattices”. Science. Vol. 287.
2000. pp. 1989-1992.
4. Q. A. Pankhurst, J. Connolly, S. K. Jones, J.
Dobson. “Applications of magnetic nanoparticles in
biomedicine”. J. Phys D: Appl. Phys. Vol. 36. 2003.
5. N. Pernicone, F. Ferrero, I. Rossetti, L. Forni, P.
Canton, P. Riello, G. Fagherazzi, M. Signoretto, F. Pinna. “Wustite as a new precursor of industrial
ammonia synthesis catalysts”. Appl. Catal. A: Gen.
Vol. 251. 2003. pp. 121-129.
6. E. H. Kim, H. S. Lee, B. K. Kwak, B. K. Kim.
“Synthesis of ferroluid with magnetic nanoparticles
by sonochemical method for MRI contrast agent”.J.
Magn. Mater. Vol. 289. 2005. pp. 328-330.
7. D. Maity, D. C. Agrawal. “Synthesis of iron oxide
nanoparticles under oxidizing environment and their
stabilization in aqueous and non-aqueous media”. J.
Magn. Mater. Vol. 308. 2007. pp. 46-55.
8. H. Zhang, R. Wang, G. Zhang, B. Yang. “A covalently
attached ilm based on poly(methacrylic acid)-capped
Fe3O4 nanoparticles”. Thin Solid Films. Vol. 429.
2003. pp. 167-173.
9. Y. Yang, L. Li, G. Chen. “Synthesis of magnetic
particles via a cationic–anionic urfactante vesicle
method”. J. Magn. Mater. Vol. 305. 2006. pp. 40-46.
10. Z. Huang, F. Tang, L. Zhang. “Morphology control and texture of Fe3O4 nanoparticle-coated polystyrene microspheres by ethylene glycol in forced hydrolysis
reaction”. Thin Solid Films. Vol.471. 2005. pp. 105-112.
11. Z. L. Liu, X. Wang, K. L. Yao, G. H. Du, Q. H. Lu, Z. H. Ding, J. Tao, Q. Ning, X. P. Luo, D. Y. Tian, D. Xi. “Synthesis of magnetite nanoparticles in W/O
microemulsion”. J. Mater. Sci. Vol. 39. 2004. pp.
12. Y. Okano, T. Nakamura. Hydrothermal synthesis of
aluminum bearing magnetite particles. Colloids and
Surfaces. Vol. 139. 1998. pp. 279-285.
13. U. Schwertmann, R. M. Cornell. Iron Oxides in the
Laboratory. Preparation and Characterization. 2a ed.
Ed. Wiley, Weinheim. 1991. pp. 75-111.
14. W. Yu, T. Zhang, J. Zhang, X. Qiao, L. Yang, Y. Liu. “The synthesis of octahedral nanoparticles of
magnetite”Mat. Lett. Vol. 60. 2006. pp. 2998-3001.
15. Y.K. Gun’ko, S.C. Pillai, D. Mcinerney, “Magnetic nanoparticles and nanoparticle assemblies from
metallorganic precursors”. J. Mater. Sci. Mater.
Electron. Vol. 12. 2001. pp. 299-302.
16. S. Franger, P. Berthet, J. Berthon. “Electrochemical
synthesis of Fe 3O 4 nanoparticles in alkaline aqueous
solutions containing complexing agents”. J. Solid
State Electrochem. Vol. 8. 2004. pp. 218-223.
17. G. Gnanaprakash, S. Mahadevan, T. Jayakumar, P. Kalyanasundaram, J. Philip , B. Raj. “Effect of initial pH and temperature of iron salt Solutions on formation
of magnetite nanoparticles”. Mat. Chem. and Phys.
Vol. 103. 2007. pp.168-175.
18. C. A. Barrero, A. L. Morales, J. Mazo-Zuluaga, F. Jaramillo, G. Pérez, D. M. Escobar, C. Arroyave, J. Tobón, P. M. Montoya, L. Ososrio, R. E Vandenberghe,
J. M. Greneche. “Synthesis and Mössbauer
characterization of Cu and Cr doped magnetites”. Rev.
Metal. Madrid. Vol. Extr. 2003. pp. 62-67.
19. J. Deng, Ch. L. He, Y. Peng, J. Wang, X. Long, P. Li,
A. S. C. Chang. “Magnetic and conductive Fe3O4–
polyaniline nanoparticles with core–shell structure”.
Synt. Met. Vol. 139. 2003. pp. 295-301.
20. P. S. Shidu, R. J.Gilkes, A. M. Posner. “The synthesis and some properties of Co, Ni, Zn, Cu, Mn and Cd
substituted magnetites”.J. inorg. nucl. chem. Vol. 40.
1978. pp. 429-435.
21. R. M. Cornell, U. Schwertmann. Iron oxide. Structure,
Properties, Reactions, Ocurrence and Uses. 2a ed. Ed.
Wiley, Weinheim. 2003. pp. 149.
22. D. K Kim, Y. Zhang, W. Voit, K. V.Rao, M. Muhammed. “Synthesis and characterization of surfactant-coated superparamagnetic monodispersed
iron oxide nanoparticles”. J. Magn. Mater. Vol. 225.
2001. pp. 30-36.
23. R. W. Chantrell, A. Bradbury, J. Popplewell, W.
Charles. “Agglomerate formation in a magnetic luid”.
J. of Appl. Phys. Vol. 53. 1982. pp. 2742-2744.
24. J. H. Wu, S. P. Ko, H. L.Liu, S. Kim, J. S. Ju, Y. K Kim. “Sub 5 nm magnetite nanoparticles: Synthesis,
microstructure, and magnetic properties”. Mat. Lett.
Vol. 61. 2007. pp. 3124-3129.
25. L. Li, Y. Chu, Y. Liu, D. Wang. “Solution-phase
synthesis of single-crystalline Fe3O4 magnetic
nanobelts”. Journal of Alloys and Compounds. Vol.